Presentation on theme: "Morphology of Nanoclusters and Nanopillars Formed in Nonequilibrium Surface Growth for Catalysis Applications V. Gorshkov 1,2, A. Zavalov 3, V. Privman."— Presentation transcript:
Morphology of Nanoclusters and Nanopillars Formed in Nonequilibrium Surface Growth for Catalysis Applications V. Gorshkov 1,2, A. Zavalov 3, V. Privman 2 1 National Technical University of Ukraine, Kiev, Ukraine 2 Center for Advanced Materials Processing, Clarkson University, USA, NY 3 Institute of Physics, National Academy of Sciences, Kiev, Ukraine Abstract We consider growth of nanoclusters and nanopillars in a model of surface deposition and restructuring yielding morphologies of interest in designing catalysis applications. Kinetic Monte Carlo numerical modeling yields examples of the emergence of FCC-symmetry surface features, allowing evaluation of the fraction of the resulting active sites with desirable properties, such as (111)-like coordination, as well as suggesting the optimal growth regimes. The work has been done by collaboration with Center for Emerging Energy Technologies, Department of Chemical and Nuclear Engineering, University of New Mexico, Albuquerque, NM 87131, USA 1
Results of this work have been highlighted by the Editors of Langmuir by using a compilation of images for a cover of Issue 13 of Volume 27.
2 Wang, CM, DR Baer, JE Amonette, MH Engelhard, Y Qiang, and J Antony. 2007. "Morphology and oxide shell structure of iron nanoparticles grown by sputter-gas-aggregation." Nanotechnology 18:255603
T here are obviously other "microscopic" parameters in the problem that can be adjusted, such as, for instance, the attachment probability of the arriving atoms, which could be made less than 1, etc. However, there are also "macroscopic" parameters, such as the geometry of the system and the lattice symmetry-related properties, that can also be modified. One important choice is that of the initial substrate for deposition. Growth of isolated nanoparticles, considered in an earlier study, yields useful insights into the problem of selecting a substrate for surface-feature formation. Specifically, in the nonequilibrium regime, nanosize shapes can be dominated, for a range of growth times and particle sizes, by densely packed faces of symmetries similar to those encountered in the Wulff construction, but with different proportions. F or FCC, the figure shows the Wulff form, involving the (100) and (111) type faces. For nonequilibrium growth, two shapes are shown. One still has the (100) and (111) faces, but in the other, formed under faster-growth conditions, the (111) faces "win" and dominate the shape. Generally, this suggests that (100) and (111) are naturally complementary lattice faces in nonequilibrium FCC-symmetry growth, and therefore (100)-consistent substrates are a good choice for growing (111), if a (111)-consistent initial surface is not an option. Similar examples for some other lattice symmetries are available. In addition to these empirical/theoretical considerations, we note that the natural emergence of octahedral shapes made of (111)- and (100)-type faces, for on-surface Pt nanoclusters, is a well established property in experiment.
Time dependence of the areal density of the approximately (111)- coordinated surface atoms, for the same growth parameters as in Figure 3. (The solid line was added for guiding the eye.) Top panel: The isolated- pyramid growth stage. Bottom panel: Illustration of growth carried out somewhat beyond the "plateau" (isolated- growth) regime. The inset diagrams highlight the locations of the hexagonal- shaped, predominantly (111) type regions near the tops of two typical peaks, marked A and B, that grew to different heights at this later growth stage.
Conclusion I n summary, we established that numerical-simulation modeling can yield interesting information on the emergence of the morphology features of growing nanostructures for applications of interest in catalysis. Specifically, growth on flat substrates is best carried out only as long as the resulting structures are isolated nanoclusters. Larger surface features, even if formed as well-defined nanopillars, are not guaranteed to have the desirable surface-face properties. W e also found that well-defined surface features are obtained for relatively narrow ranges of parameter values, for those quantities which, here loosely, are related to the on-surface diffusion rate and to temperature. F uture studies might explore approaches such as seeding/templating, in order to grow larger (taller) surface features potentially offering larger exposed area with preferred symmetry, such as (111). Furthermore, with substantially more powerful numerical resources invested, it should be possible to carry out realistic simulations with the actual material parameters, as well as for new materials of interest in applications.
Your consent to our cookies if you continue to use this website.